Micro Tensile Tester
BISCO, Inc. • 1100 W. Irving Park Rd. • Schaumburg, IL 60193 • U.S.A. • 847-534-6000 • www.bisco.com
Made in the U.S.A.
Rev. 10/08 1 of 9
MICRO TENSILE TESTER
MICRO TENSILE TESTER USER INSTRUCTIONS
The Bisco Micro Tensile Tester (MTT) is designed to test 1mm x 1mm (approx.) cross sectional samples of composite bonded to tooth.
The typical force required for testing is less than 45 lbs., 20 kg or 200 newtons.
WARNING: Safety glasses should be worn when using the MTT or preparing samples for testing.
CAUTION: Do not exceed the maximum force limit of the force gauge supplied or irreversible damage to the force gauge
The shipment should contain the following items. Please do not discard the shipping carton until all items have been
1. 1 Test bed – black anodized square channel 4” x 4” x 18.6 “ long with electronics control panel attached
2. Box contains 1 force gauge assembly – the contents listed on the box as it comes from the manufacturer have been
modified by BISCO to assemble the force gauge to be used on the MTT. There will only be one item in the box, but it
is the complete assembly as needed for use with the MTT
3. 1 AC to DC power adapter
4. Test block assemblies in clear plastic protective tube
5. 10 Polycarbonate introductory kit blocks for holding and cutting sample bars
6. 1 Zapit* introductory kit
7. Blue tinted core material (2 Syringes, 2.5g ea.)
1. Place the MTT on the bench with the control panel
facing the user.
2. Place the force gauge assembly on the test bed by
positioning the 4 notches in the slide plate over the
4 slide shoulders. See Figure 1.
Rest the bottom of the slide plate on the test bed, then
slide to the left so the plate is held under the shoulders.
See Figure 2.
3. The pull block should be slightly loose. See Figure 2.
4. Slide the gauge assembly further to the left and place
the nylon strap over the motor CAM. See Figure 3.
2 of 9
3 *Zapit Base, Zapit Accelerator, and Zapit Solvent are available from Dental
Ventures of America, 800-2280-6696, www.dentalventures.com as well as
BISCO (see ACCESSORIES).
5. Plug the cord on the back of the test bed into the
power jack on the force gauge located on the right
side of the gauge. See Figure 4.
6. Plug the cord from the AC adapter into the jack on
the left side of the control panel. See Figure 5.
7. Plug the AC adapter into the wall socket. The tester
is now powered.
8. Turn on the force gauge by pressing the On/Zero
button. Allow the force gauge to perform its power-on
self-test sequence. For best results, hold the On/Zero
button until the display reads no AO (“No Auto Off”).
9. The force gauge is factory set to store and display the
maximum tensile force in kilogram units. This is
indicated by two vertical arrows in opposite directions
and “MAX” on the left side of the display and “kg”
in the middle of the display. To change the desired
measurement units and gauge mode, refer to the
FORCE GAUGE INSTRUCTIONS included in this
10. The unit is ready for use.
11. The unit has a variable speed control. In the nominal
position the force is applied such that a typical
sample will break in about 60 seconds. The speed can
be adjusted faster (+) or slower (-) than nominal. The
speed is determined by the voltage applied to the
CAM motor. Although the unit is not calibrated for
speed, the same speed can be set and repeated by
measuring the voltage to the motor with the two test
jacks on the right side of the control box.
To determine the motor voltage, plug the pin probes
typically used with a digital voltmeter into the jacks
on the right side of the control panel. See Figure 6.
Set the meter for 20 volts DC. Before mounting a
sample to the tester, run the unit by pressing the start
button. When the motor is running, measure and
record the voltage reading. The voltage can be
adjusted while the motor is running during the
voltage setting process, (but it is not recommended to
vary the speed during actual testing.) Once the voltage
is set, the testing may be performed.
NOTE: The speed that the unit resets at (clockwise
rotation) is not the same speed that the unit performs
the tests at (counterclockwise).
3 of 9
DESCRIPTION OF TEST BLOCK
SUGGESTED PREPARATION OF SAMPLE AND TEST BLOCK
4 of 9
1. The test block is a precision machined assembly
providing a minimum of play between the test jaws
while also minimizing the friction between the jaws.
See Figure 7.
2. Care should be taken when storing and handling to
keep the block clean as to avoid any possible damage.
Do not twist or bend the brass slide keys, as this will
cause the test block to bind and give erroneous
3. The jaws of the test block have a 2mm gap between
them to allow the test sample to be glued to the block
without glue migrating between the jaws and giving
erroneous readings. The edges of the jaws are also
cut back at an angle to further allow the sample to be
glued in place without glue dripping between the
jaws. See Figure 8.
4. The test block is made from steel for durability.
Broken samples and adhesive can be removed by
scraping with the edge of a sharp razor blade.
5. Do not clean the test block with abrasive powders,
acidic or alkaline cleaning agents.
6. Some users find it convenient to have two test block
assmblies to allow one to be prepared while the other
is being used on the test bed.
1. Prepare a flat dentin surface perpendicular to the occlusal direction using a slow speed diamond cutting wheel or a
grinding wheel and water cooling.
2. Create a smear layer by abrading the surface with wet silicon carbide paper. 320 grit is suggested for self-etched
adhesives and 600 grit is suggested for total-etch adhesives.
3. Flatten the gingival side of the sample on a grinding wheel and attach to a mounting block (acrylic or polycarbonate)
with KERR Sticky Wax. Recommended block size is 1.5” x .75” x .4“. Mounting blocks are available from BISCO (see
4. Apply and cure a layer of adhesive per manufacturer’s instructions.
5. Apply and cure 1 or 2 layers of composite per manufacturer’s instructions, up to a maximum of about 4mm thickness.
A special blue tinted core material is available from BISCO allowing the interface between the dentin and composite
to be easily seen (see ACCESSORIES). After a sample is broken, it should be inspected to verify that the break
occurred at the composite/adhesive/dentin interface rather than the composite or dentin. If a break occurred other
than at the interface, the user should decide how to include the results in the data. If there is white and blue material
on a section of broken test sample, the break did not occur at the interface.
6. Soak the sample for 24 hours at 37° C to optimize the cure and bond.
7. Section into 0.9mm thick slabs from the occlusal to
the gingival using a water cooled diamond saw at
100rpm with 75 grams of force.
Tip: Move the saw index 0.9mm plus the width of the
blade each time. See Figure 9. Make sure the cuts are
perpendicular to the bond interface.
8. Mount the slab sections flat on their side onto another
plastic block with KERR Sticky Wax and section into
0.9mm x 0.9mm bars. See Figure 10. It is important to
make sure that the bars are cut such that the bond
interface is perpendicular to the sides. If not, the cross
section area will be slightly larger as it will be a
diagonal across the measured bar dimensions and
the force applied will not be perpendicular to the
bond, resulting in an invalid computation of MP as
well as some shear force vectors instead of pure
tensile force acting on the bond interface.
9. Let the bars soak in room temperature DI water until
ready for mounting to the test block.
10. Break away the wax at each end of the array of bars
and carefully pick one bar off the block with the end
of a scalpel. See Figure 11.
11. Scrape any excess wax from the samples and
measure the actual cross sectional dimensions of the
sample and record.
Tip: Scrape towards the interface rather than away
so as not to put any stress on the interface and break
12. Place the sample on a paper towel to absorb any
13. Make sure the surface of the test block is clean and
free of material from the previous test. The jaws
should be off of the test bed on the bench, on a paper
towel or sheet of rubber.
14. Close the jaws tightly together. Place a drop of glue
(Zapit Base*) on each jaw in the middle of the test
sample mount area. See Figure 12.
15. Pick up the sample with tweezers at the interface and
place on the jaws. It is important that the samp